polymerization of peptide polymers for biomaterial applications
Post on 06-Feb-2017
Embed Size (px)
2013 Baker and Numata, licensee InTech. This is an open access chapter distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Polymerization of Peptide Polymers for Biomaterial Applications
Peter James Baker and Keiji Numata
Additional information is available at the end of the chapter
1. Introduction The term biomaterial, as defined by a consensus conference on Definitions in Biomaterial Science, is a material intended to interface with biological systems to evaluate, treat, augment or replace any tissue, organ of function of the body.  Biomaterials range from the simple embedded material to complex functional devices. There are three primary types of biomaterials: 1) metallic, based on metallic bonds, 2) ceramic, based on ionic bonds, and 3) polymeric, based on covalent bonds.  Polymers that are mechanical resistance, degradable, permeable, soluble and transparent, have been used in both simple and complex biomaterial applications. [3-5] The mechanical properties of poly(esters), poly(amides), poly(amidoamines), poly(methyl methacrylate), and poly(ethyleneimine), are particularly well suited (Table 1). These polymeric materials have given rise to first and second-generation biomaterials.  Next-generation biomaterials will have less toxic degradation products, undergo hierarchal assemble to form supramolecular structures, and maintain a sustainable design. The degradation products of synthetic polymers are of acidic and cannot be metabolized biological systems. This can result in a bioaccumulation of these products offsetting the homeostatic balance of the system. The production of synthetic polymers requires bulk separation and crystallization, which often inhibits the formation of higher ordered structures. Finally, the source materials for these polymers are petrochemicals. The dependency on petrochemicals presents both environmental and sustainability concerns. The development of materials that overcome these limitations would be a significant advancement in the field of biomaterials.
Biological materials have capabilities that far exceed those which are synthesized chemically. [21, 22] Biopolymers including polypeptides, can serve as replacement materials for synthetic polymers. Polypeptides such as collagen, elastin, and silk, are currently being sought as next-generation biomaterials (Table 2). [23-28] Collagen, a major constituent of bone, cartilage, tendon, skin and muscle, are the most abundant proteins in the human body.  Several
Polymer Science 230
different types of collagen have been identified; these proteins are distinguished by their triple-helical structure. Type I collagen forms supramolecular assemblies. This assembly is controlled by environmental parameters such as concentration, pH, and ionic strength, making it of particular interest as a biomaterial.  Type I collagen is approximately 1000 amino acids long and contains a tripeptide (-Pro-Hyp-Gly-)n tandem repeat, where Hyp is a postranslationally modified hydroxyproline. Elastin is an extracellular matrix protein responsible for the extensibility and elastic recoil of blood vessels, ligaments and skin. Elastin is approximately 70 kDa protein composed of crosslinking domains and elastin domains. Elastin domains are composed poly(Gly-Val-Gly-Val-Pro)n and poly(Gly-Val-Gly-Val-Ala-Pro)n of repeating sequences. These domains undergo an inverse temperature transitions where the protein forms a crystalline state on raising the temperature and redissolve on lowering the temperature. [30, 31] Silks are fibrous proteins spun by silkworms and spiders. They have a range of functions, including cocoons to protecting eggs or larvae, draglines to support spiders, and the formation of webs that can withstand high impacts of insect prey.  The mechanical strength of dragline spider silks has led to its employment in several biomedical applications. Dragline spider silk is around 300 kDa protein composed of two repeating domains: poly(Ala)n and poly(Gly-Gly-Gly-Xaa-Gln-Tyr)n, where Xaa can be any amino acid. The strength of this polymer is a result of the highly crystalline structure of the poly(Ala) domains and the amorphous poly(Gly-Gly-Gly-Xaa-Gln-Tyr) repeat is amorphous in structure which allows for flexibility. [33, 34] All of three of these high molecular weight polypeptides are composed of highly repetitive amino acid sequences. The present review will be concerned with the synthesis of polypeptides and how they polypeptides will be used in the production of new biomaterials.
Polymer Biomaterial Application Ref Synthetic Polymer Polyester Drug Delivery, Sutures, Stents, Nanoparticles [7-10] Polyamides Sutures, Wound Dressings  Polyamidoamine Biomedical Imaging  Poly(methyl methacrylate) Contact Lens  Polyethyleneimine Gene Delivery, Tissue Engineering [13-15] Natural Polymer Polypeptides Gene Delivery, Biomedical Imaging, Drug Delivery, [16-18] Polysaccharides Tissue Engineering, Nanoparticles  Polynucleotide Biomedical Imaging 
Table 1. Survey of synthetic and natural polymers used as biomaterials
Polypeptide Repeating Sequences MW (kDa) Ref Collagen (-Pro-Hyp-Gly-) n ~ 400 
Elastin (-Gly-Val-Gly-Val-Pro-) n, or (-Gly-Val-Gly-Ala-Pro-) n ~ 70 [30,31]
Spider Silk (-Ala-)n or (-Gly-Gly-Gly-Xaa-Gln-Tyr-) n ~ 300 [33,34]
Table 2. Amino acid sequence of polypeptides being used as biomaterials
Polymerization of Peptide Polymers for Biomaterial Applications 231
The synthesis of polypeptides means formation of amide bonds between amino acid monomers. Amide bonds are formed by a condensation reaction between a carboxylic acid and an amine. The conventional chemical method for amide bond synthesis requires the activation of the carboxyl group followed by a nucleophilic attack by a free amine. This requires the presence of coupling reagents, base and solvents (Figure 1A).  When this condensation reaction occurs between two amino acids the resulting amide bond is a peptide bond. Solid phase peptide synthesis (SPPS), developed by Merrifield, provides a fast an efficient manner to synthesis polypeptides. In SPPS, the N-terminal amino acid is attached to a solid matrix with the carboxyl group and the amine group is protected (Figure 1B). Amine group undergoes a deprotection step revealing an N-terminal amine. This is followed by a coupling reaction between the activated carboxyl group of the next amino acid and the amine group of the immobilized residue. Side chains of several amino acids contain functional groups, which may interfere with the formation of amide bonds and must be protected. This process may continue through iterative cycles until the polypeptide has reached its desired chain length. Polypeptide is then cleaved off the resin and purified. [35-37] SPPS has enabled the synthesis of ogliopeptides ~40 to 50 amino acids residues. However, limitations in chemical coupling efficiency have made it impractical to synthesize longer polypeptides with reasonable yields.
Figure 1. Chemical synthesis of polypeptides. A) The chemical synthesis of an amide bond requires the activation of the carboxylic acid B) Solid phase peptide synthesis.
Polymer Science 232
Peptide bonds, the key chemical linkage in proteins, are synthesized not only chemically but also biologically. In this process the primary structure of a protein is encoded in a gene, a short sequence of deoxyribonucleic acid (DNA). A two-step process of transcription and translation are required to biosynthetic extract this information from a gene. Transcription is the step where the genetic information encoded from the DNA is transcribed into messenger ribonucleic acid (mRNA) in the form of an overlapping degenerate triplet code. This process occurs in three stages: initiation, chain elongation, and termination. Initiation occurs when the RNA polymerase binds to the promoter gene sequence on the DNA strand. Elongation begins as the RNA polymerase is guided along the template DNA unwinding the double-stranded DNA molecule as well as synthesizing a complementary single-stranded RNA molecule. Finally, transcription is terminated with the release of RNA polymerase from template DNA. Translation involves the decoding of the mRNA to specifically and sequentially link together amino acids in a growing polypeptide chain. Decoding of mRNA occurs in the ribosome, a macromolecular complex composed of nucleic acids and proteins. mRNA is read in three-nucleotide increments called codons; each codon specifies for a particular amino acid in the growing polypeptide chain (Figure 2). Ribosomes bind to mRNA at the start codon (AUG) that is recognized by initiator tRNA. Ribosomes proceed to elongation phase of protein synthesis. During this stage, complexes composed of an amino acid linked to tRNA sequentially bind to the appropriate codon in mRNA by forming complementary base pairs with the tRNA anticodon. Ribosome moves from codon to codon along the mRNA. Amino acids are added one by one, translated into polypeptide sequences dictated by DNA and represented by mRNA. At the end, a release factor binds to the stop codon, terminating translation and releasing the complete polypeptide from the ribosome.
Figure 2. Cartoon representation of polypeptide synthesis on the ribosome.
Polymerization of Peptide Polymers for Biomaterial Applications 233
The advent of recombinant DNA technology has allowed the facile, large-scale production of many polypeptide sequences. However, polypeptides containing highly repetitive seq